2 Wydano za zgodą Rektora R e d a k t o r n a c z e l n y Wydawnictw Politechniki Rzeszowskiej prof. dr hab. inŝ. Leonard ZIEMIAŃSKI R a d a N a u k o w a ZN PRz Mechanika Sergei ALEXANDROV (Rosja), Józef GAWLIK, Rudolf KAWALLA (Niemcy), Krzysztorf KUBIAK, Thomas G. MATHIA (Francja), Tadeusz MARKOWSKI, Pavlo MARUSCHAK (Ukraina), Paweł PAWLUS, Andrea PICCOLROAZ (Włochy), Marderos Ara SAYEGH (Syria), Jarosław SĘP, Emil SPISǍK (Słowacja), Feliks STACHOWICZ, Marian SZCZEREK, Nicolae UNGUREANU (Rumunia) K o m i t e t R e d a k c y j n y redaktor naczelny prof. dr hab. inŝ. Feliks STACHOWICZ redaktorzy tematyczni (naukowi) dr hab. inŝ. Krzysztof KUBIAK, prof. PRz dr hab. inŝ. Jarosław SĘP, prof. PRz dr hab. inŝ. Andrzej TOMCZYK, prof. PRz redaktor statystyczny prof. dr hab. inŝ. Paweł PAWLUS sekretarz redakcji dr inŝ. Tomasz TRZEPIECIŃSKI członkowie dr hab. inŝ. Grzegorz BUDZIK, prof. PRz dr inŝ. Tadeusz BALAWENDER R e d a k t o r z y j ę z y k o w i Marta JAGIEŁOWICZ Natalia TRZEPIECIŃSKA P r z y g o t o w a n i e m a t r y c Joanna MIKUŁA p-issn e-issn Wersja drukowana Kwartalnika jest wersją pierwotną Recenzenci współpracujący 2012 r. s. 73 Oficyna Wydawnicza Politechniki Rzeszowskiej al. Powstańców Warszawy 12, Rzeszów Nakład 130 egz. Ark. wyd. 4,38. Ark. druk. 4,75. Papier offset. kl. III 70g B1. Oddano do druku w grudniu 2012 r. Wydrukowano w styczniu 2013 r. Drukarnia Oficyny Wydawniczej, al. Powstańców Warszawy 12, Rzeszów Zam. nr 137/12
3 SPIS TREŚCI Paweł FROŃ, Feliks STACHOWICZ Bending force and springback characteristics of the Tailor-Welded 18G2A-E355 steel strips... 5 Marek KROK, Janusz PORZYCKI, Roman WDOWIK Parametryczne programowanie szlifowania wyrobów ceramicznych o zło- Ŝonej geometrii Andrzej SKRZAT Application of coupled Eulerian-Lagrangian approach in metal forming simulations Ján SLOTA, Miroslav JURČIŠIN Experimental and numerical analysis of the deep drawing process using optical measuring system Roman ŠÚŇ, Emil SPIŠÁK Evaluation of the cutting edge fan-shaped during the cutting process by the hydro abrasive water jet Tomasz TRZEPIECIŃSKI Advances in sheet metal forming technologies Recenzenci współpracujący 2012 r
5 ZESZYTY NAUKOWE POLITECHNIKI RZESZOWSKIEJ Nr 284 Mechanika z. 84 (4/12) 2012 Paweł FROŃ REMET S.A., Stalowa Wola Feliks STACHOWICZ Rzeszow University of Technology BENDING FORCE AND SPRINGBACK CHARACTERISTICS OF THE TAILOR-WELDED 18G2A-E355 STEEL STRIPS In many studies a wide range of information about the bendability, failure patterns and the springback of homogeneous as well as tailor-welded sheet metal parts are presented. However, accurate prediction of the springback remains elusive, especially in the case of thick sheet metal. The purpose of this study was experimental determination of the bending force and springback coefficient of the tailor-welded 18G2A-E355 steel strips. Especially, it was focused on comparing the differences in the mechanical properties and bending characteristics between the tailor-welded strips and non-welded ones under the same experimental conditions. The set-up mounted on the testing machine, instrumentation and process control system allows the rig to operate in displacement as well as load control. The MAG method with the Argon + CO 2 atmosphere was used for strips welding. Keywords: tailor-welded sheet metal, strain hardening, bending force, springback 1. Introduction Bending is one of major sheet and strips forming operations widely used in modern industries. For this reason, understanding the bending process helps to provide some information crucial to industrial production. Recently many industry companies are trying to form different products by using tailor-welded blanks. A tailor-welded blank consists of two or more sheets that have been welded together in a single plane prior to forming. And the sheets joined by welding can be identical, or they can have different thickness, mechanical properties or surface coatings. Various welding processes, i.e. laser welding, mash welding, electron-beam welding or induction welding, can join them. In the field of sheet metal bending, one can find literature on pure bending, V-die bending, simple flanging and so on. Most materials can be bent to quite a small radius, but a problem is to control the shape of the bend workpiece. In general, a bend workpiece will recover elasticity i.e. springback on unloading, so
6 6 P. Froń, F. Stachowicz that the bend quality is heavily dependent on the springback, which is a function of material properties and process parameters such as Young s modulus, yield stress, strain hardening abilities, plastic anisotropy, thickness and die geometry [1-6]. The most important die bending process is bending in a V-shaped die, so that deformed shape results from the sheet being pressed into the die by the punch until it is in contact with the sides of the die to the maximum extent possible. Springback is a phenomenon in which the metal strip unbends itself after a forming operation. Control of springback for the bending processes applied in practice is difficult for a number of reasons, especially in mass production [2, 7-12]. In the case of tailor-welded strips the quality of the weld is critical for a successful forming operation [13, 14] and affects springback phenomenon [15, 16]. Sheet metal forming processes, such as bending, stretching and drawing are widely applied industrially, but design of tools and selection of sheet material remain almost invariably dependent on trial and error . The main reason is that the shape of tools, characteristics of material, process variables and the geometric configuration of the workpiece all influence the manufacturing process: these characteristics are difficult to formulate into a precise mathematical model. The evaluation of elastic springback effects is a fundamental aspect in the practice of sheet forming operations. Springback, in fact, introduces deviations from the desired final shape consequently, the stamped sheet does not conform to the design specifications and could result in being unsuitable for the application. A complete knowledge of the springback phenomenon and its dependence on material and process variables is strongly required in order to develop effective real time process control systems. The main purpose of this study was experimental determination of the bending force and springback coefficient of the tailor-welded 18G2A-E355 steel strips. Especially, it was focused on comparing the differences of the mechanical properties and bending characteristics between the tailor-welded strips and nonwelded ones under the same experimental conditions. 2. Experimental materials and methods The 18G2A-E355 steel strips, 9.0 mm thick were used in this experiment. The MAG method with the Argon + CO 2 atmosphere was used for strips welding. Geometry of strip edge prepared for welding is presented in Fig. 1. When the mechanical testing is concerned, 3 types of tensile specimens (Fig. 2) of 240 mm gauge length and 12.5 mm width in gauge region were prepared from: based material strip, strip containing longitudinal weld, strip containing transverse weld.
7 Bending force and springback... 7 The experiments were carried out using a special device, which recorded simultaneously the tensile load, the current length of the specimens. Fig. 1. Geometry of strip edge prepared for welding a) b) c) Fig. 2. Tensile specimens with longitudinal weld (a), transverse weld (b) and base material (c) For many years strain hardening laws such as those from Ludwig, Hollomon, Voce, Swift and Krupkowski have been used to describe the plastic behaviour of polycrystalline metals and alloys. The Hollomon law in the form of: σ ε n = C (1) has been used the most frequently. The parameters involved in this law, particularly n-value have been correlated to changes in the microstructure of a material and in some way represent processes, which occur during deformation. They have also been used extensively to characterise the formability of sheet material. The value of strain hardening exponent, n, is usually determined from the double logarithmic plot of the true stress and true strain by linear regression.
8 8 P. Froń, F. Stachowicz A of bending experiments have been used to reveal bending characteristics of sheet metals. Most of such tests use two-dimensional geometry for simplified analysis and the simulation, while also being a representative of many industrial parts. In the case of our experimental investigation three rolls bending test was used (Fig. 3). The set-up mounted on the testing machine, instrumentation and process control system allows the rig to operate in displacement as well as load control. As in tensile testing three types of specimens 25 mm wide were deformed: continuously to determine bending force characteristic, progressively to determine springback characteristic loaded and unloaded by suitable punch motion up to nearly 70 mm deflection. The specimen shape at corresponding bending stage was recorded using the digital photo-camera and stored as.jpg files. Using professional computer code GIMP, the.jpg files were elaborated in order to determine changes in a specimen shape, caused by springback phenomenon, and then the springback coefficient was calculated as: R R a K = (2) s where: R a radius in active phase of bending (under pressure), R s radius in passive phase of bending (after springback). Fig. 3. Scheme of the three rolls bending test 3. Results and discussion The results of uniaxial tensile of the 18G2A-E355 steel strips (Table 1 and Fig. 4) demonstrate the visible effect of weld presence in the tested specimen. In comparison with base material characteristic, in the case of welded material characteristic it could be noticed that:
9 Bending force and springback... 9 the presence of weld reduces the value of both the uniform and total elongation, especially in the case of the specimen with transverse weld, the value of ultimate strength of specimen with longitudinal weld are higher while that of the specimen with transverse weld are smaller, the presence of weld resulted in smaller value of the strain hardening exponent. Table 1. Mechanical properties of the 18G2A-E355 steel specimens Specimen type R e [MPa] R m [MPa] A 50 [%] C [MPa] Base material Longitudinal weld Transverse weld n 600 stress [MPa] Stress, MPa without weld longitudinal weld transverse weld 0 0 0,05 0,1 0,15 0,2 0,25 elongation Elongation Fig. 4. Flow characteristics of the 18G2A-E355 steel specimens The highest value of the yield stress and ultimate strength in the case of longitudinal weld resulted from the presence of hard material zone in the centre of weld along the whole specimen in loading direction. The lowest value of the ultimate strength as well as ultimate strain resulted from the presence of two weak material zones located near the weld and oriented transverse to specimen loading. It was confirmed by the strain localisation and specimen failure closed to the weld region.
10 10 P. Froń, F. Stachowicz The bending characteristics, i.e. the relation between bending force and curvature, demonstrate similar run, both in the case of the base material specimen and specimen with longitudinal or transverse weld (Fig. 5). At the first elastic stage of bending, the bending force increases linearly with curvature increase. At the elastic-plastic range of bending the bending force still increases with bending curvature due to strain hardening of a material, and reaches its maximum. At the next stage the bending force started to decrease, as a result of crosssection reduction. The presence of the weld resulted in bending force increasing in the whole range of curvature. This effect is more visible in the case of specimen with longitudinal weld. For the strip with transverse weld the intensity of bending force decrease at the last stage of bending was the most visible. bending force Bending [kn] force, kn longitudinal weld transverse weld without weld deflection Deflection, [mm] Fig. 5. Bending force characteristics of the 18G2A-E355 steel specimens The results of springback coefficient calculation were plotted as a function of bending radius (under loading), it means as springback characteristic (Fig. 6). From this presentation it is visible that the value of springback coefficient increases with bending process proceeding, what is a result of elastic zone decreasing in the centre of sheet thickness. The visible change in the springback charecteristic position in comparison with the base material specimen was observed in the case of specimen with longitudinal weld. The presence of transverse weld resulted in slightly larger springback phenomennon, it means smaller value of springback coefficient. The visible change in springback characteristic in the case of the specimens with longitudinal weld in comparison with that of based material resulted mainly
11 Bending force and springback from the presence of hard material zone in the centre of weld located along whole specimen length and oriented along the bending curvature. In the case of the transverse weld, lower values of the springback coefficient in comparison with that of the based material are observed. It seemed to be the result of transverse orientation of the weld (with one hard and two weak material zones) according to the bending curvature and the location of the weld in the region of the bending punch nose. K 1,0 0,8 K 0,5 0,3 without weld transverse weld longitudinal weld bendin Bending radius radius, [mm] mm Fig. 6. Springback characteristic of the 18G2A-E355 steel specimens 4. Conclusion As it should be expected the presence of welding zone in the tested material has the visible effect on both the tensile flow and bending characteristics. The presence of the weld resulted in the bending force increase in the whole range of curvature especially in the case of the specimen with longitudinal weld. Taking into account the springback phenomenon in the case of longitudinal weld this effect could be treated as positive, mainly due to higher value of the springback coefficient in the whole range of bending radius. The presence of transverse weld resulted in decrease of flow characteristic as well as the springback phenomenon is more visible in comparison with the base material (the specimen without any weld). References  Marciniak Z.: Mechanika procesów tłoczenia blach, WNT, Warszawa  Lange K.: Handbook of metal forming, McGraw-Hill Company, New York 1985.
12 12 P. Froń, F. Stachowicz  Świątkowski K., Stachowicz F.: Analysis of the cross-sectional deformation of box profiles subjected to bending, J. Mech. Work. Technol., 10 (1984),  Stachowicz F.: Bending with upsetting of copper tube elbows, J. Mech. Work. Technol., 100 (2000),  Stachowicz F., Litwin P., Frącz W.: Experimental and numerical study of open structural profile bending process, Arch. Metall. Mat., 50 (2005),  Huang Y-M., Leu D-W.: Effects of process variables on V-die bending process of steel sheet, Int. J. Mech. Sci., 40 (1998),  Krywult B., Kawalec S., Stachowicz F.: Automatyczna korekcja krzywizny materiału przy gięciu spręŝysto-plastycznym, Mechanik, 53 (1980),  Lee S.W., Yang D.Y.: An assessment of numerical parameters influencing springback in explicit finite element analysis of sheet metal forming process, J. Mech. Work. Technol., 80-81, 1998,  Stachowicz F.: Experimental and numerical study springback problems in sheet metal bending, Arch. Metall., 48 (2003),  Frącz W., Stachowicz F.: Springback phenomenon in sheet metal V-die air bending experimental and numerical study, Manuf. Eng., 7 (2008),  Chalal H., Racz S-G., Balan T.: Springback of thick sheet AHSS subjected to bending under tension, Int. J. Mech. Sci., 59 (2012),  Lim H., Lee M.G., Sung J.H., Kim J.H., Wagoner R.H.: Time-dependent springback of advanced strength steels, Int. J. Plasticity, 29 (2012),  Abdullah K., Wild P.M., Jeswiet J.J., Ghasempoor A.: Tensile testing for weld deformation properties in similar gage tailor welded blanks using the rule of mixtures, J. Mech. Work. Technol., 112 (2001),  Sunar M., Yilbas B.S., Boran K.: Thermal and stress analysis of a sheet metal in welding, J. Mech. Work. Technol., 172 (2006),  Chang S.H., Shin J.M., Heo Y.M., Seo D.G.: J. Mech. Work. Technol., (2002),  Daxin E., Liu Y.: Springback and time-dependent springback of 1Cr18Ni9Ti stainless steel tubes under bending, Materials Design, 31 (2010), Experiments were performed using aperture completed thanks to financial support of UDA-RPPK /10 and POPW /09-00 and co-financed by the European Union from the European Regional Development Fund within Regional Operational Programme for the Podkarpackie Region for the years SIŁA GIĘCIA ORAZ SPRĘśYNOWANIE W PROCESIE GIĘCIA SPAWANYCH PASM ZE STALI 18G2A-E355 S t r e s z c z e n i e W wielu opracowaniach moŝna znaleźć znaczną liczbę informacji dotyczących moŝliwości gięcia, rodzaju uszkodzeń oraz spręŝynowania w procesie gięcia blach jednorodnych oraz łączonych przez spawanie. JednakŜe dokładne określenie wielkości powrotnych odkształceń spręŝys-
13 Bending force and springback tych nadal wymaga dalszych badań, szczególnie w przypadku gięcia blach grubych. Celem prezentowanych badań eksperymentalnych było określenie siły oraz współczynnika spręŝynowania podczas gięcia spawanych pasm ze stali 18G2A-E355. W szczególności skoncentrowano się na porównaniu róŝnic właściwości mechanicznych oraz charakterystyk gięcia blach jednorodnych oraz spawanych uzyskanych w takich samych warunkach testów. Przyrząd do gięcia zamontowany na maszynie wytrzymałościowej, czujniki oraz system pomiarowy umoŝliwiały rejestrację przemieszczenia oraz siły gięcia. Spawanie pasm blach przeprowadzono metodą MAG w atmosferze CO 2. Słowa kluczowe: blachy łączone spawane, umocnienie odkształceniowe, siła gięcia, spręŝynowanie DOI: /rm
15 ZESZYTY NAUKOWE POLITECHNIKI RZESZOWSKIEJ Nr 284 Mechanika z. 84 (4/12) 2012 Marek KROK Janusz PORZYCKI Roman WDOWIK Politechnika Rzeszowska PARAMETRYCZNE PROGRAMOWANIE SZLIFOWANIA WYROBÓW CERAMICZNYCH O ZŁOśONEJ GEOMETRII Wytwarzanie wyrobów z ceramiki technicznej o złoŝonej geometrii wymaga zastosowania maszyn CNC o określonych moŝliwościach technologicznych, specjalnych narzędzi ściernych oraz właściwie opracowanych programów sterujących. W artykule pokazano parametryczne programowanie obróbki przedmiotów wykonanych z ceramiki technicznej na szlifierce do wałków z osią C sterowaną numerycznie. Przedstawiono równieŝ analizę czasu obróbki typoszeregu części o sparametryzowanej geometrii. Słowa kluczowe: programowanie parametryczne, szlifowanie, szlifierka CNC, wyroby ceramiczne 1. Wprowadzenie Zapotrzebowanie na wyroby ceramiczne o złoŝonej geometrii prowadzi do potrzeby doskonalenia maszyn technologicznych sterowanych numerycznie oraz realizowanych na nich procesów obróbki. PoniewaŜ obróbka ceramiki technicznej po końcowym spieczeniu (rys. 1.) jest moŝliwa przez zastosowanie procesów obróbki ściernej, doskonalenie tych procesów staje się istotnym zagadnieniem współczesnej technologii obróbki ceramiki [1-3]. Ze względu na duŝy popyt ze strony krajowych i zagranicznych przedsiębiorstw na ceramiczne części maszyn o złoŝonych kształtach (rys. 2.), przy braku wytycznych prowadzenia obróbki, oraz potrzebę podnoszenia efektywności (w tym wydajności) procesów, przed przedsiębiorstwami związanymi z produkcją ceramicznych części maszyn są stawiane wyzwania technologiczne polegające na opracowaniu i wdraŝaniu właściwych technologii, które umoŝliwią reagowanie na potrzeby rynku oraz spowodują ich dalszy rozwój.
16 16 M. Krok, J. Porzycki, R. Wdowik Rys. 1. Przebieg procesu technologicznego dla wyrobów ceramicznych Fig. 1. The course of technological process of ceramic products Rys. 2. Przykłady ceramicznych wyrobów o złoŝonej geometrii, opracowano na podstawie  Fig. 2. Examples of ceramic products with complex geometry, prepared on the basis of  2. Wytwarzanie wyrobów z ceramiki na szlifierce CNC do wałków Przykładem wyrobów ceramicznych, których produkcja seryjna lub wielkoseryjna moŝe w niedalekiej przyszłości osiągać znaczące wyniki, są przedmioty z owalnym zarysem przekroju. Są one wykonywane na szlifierkach do wałków
17 Parametryczne projektowanie szlifowania 17 (rys. 3.), których kinematyka umoŝliwia sterowanie ruchem punktu charakterystycznego ściernicy względem układu współrzędnych przedmiotu w osiach prostoliniowych X i Z oraz osi obrotowej C (rys. 5.). WaŜnym zagadnieniem w produkcji wyrobów ceramicznych jest konieczność efektywnej obróbki części podobnych, tzn. typoszeregu wyrobów o róŝnych wymiarach. Rysunek 3. przedstawia przykładowy przedmiot obrabiany z ceramiki technicznej, który moŝe stanowić wybrany element z typoszeregu wymiarowego pokazanego na rys. 6. Rys. 3. Przykładowy przedmiot obrabiany z ceramiki technicznej Fig. 3. Example of a workpiece made of technical ceramic 3. Szlifierka CNC RUP 28 z układem Sinumerik 840Di W Katedrze Technik Wytwarzania i Automatyzacji Politechniki Rzeszowskiej została wdroŝona (w 1992 r.) szlifierka typu RUP 28 z prototypowym polskim układem CNC NUMS 740. WdroŜenie szlifierki było wynikiem realizacji wielu prac w ramach CPBR 6.1 cel Aby moŝliwe było wykorzystanie szlifierki RUP 28 do prac badawczych i produkcyjnych, konieczna była jej modernizacja (ze względu na przestarzały układ sterujący) i zastosowanie nowoczesnego układu CNC. Do sterowania obrabiarki wykorzystano układ CNC Sinumerik 840Di (rys. 4.), który umoŝliwia sterowanie osiami prostoliniowymi X i Z oraz osią obrotową C (rys. 5.).
18 18 M. Krok, J. Porzycki, R. Wdowik Rys. 4. Szlifierka RUP 28 z układem CNC Sinumerik 840Di Fig. 4. RUP 28 grinding machine with CNC Sinumerik 840Di control a) b) Rys. 5. Obróbka z osią maszynową Cm na szlifierce RUP 28 CNC: a) osie maszynowe i układy współrzędnych, b) zasada obróbki konturu podczas sprzęŝenia osi maszynowych Xm i Cm Fig. 5. Machining with Cm machine axis on RUP 28 CNC grinding machine: a) axes and coordinate systems, b) principle of contour machining (coupling of Xm and Cm axes)
19 Parametryczne projektowanie szlifowania Programowanie obróbki typoszeregu wyrobów o sparametryzowanej geometrii 4.1. Typoszereg wymiarowy wyrobów ceramicznych Przykładowy typoszereg wymiarowy wyrobów ceramicznych (odniesiony do przedmiotu z rys. 3.) przedstawia rys. 6. Dwanaście wyrobów (od M1 do M12) róŝni się promieniem zaokrąglenia części środkowej (od R13 do R2), co diametralnie zmienia kształt wyrobów i wpływa znacząco na przebieg procesu obróbki. Rys. 6. Typoszereg wymiarowy wyrobów ceramicznych Fig. 6. Type dimension of ceramic products 4.2. Sparametryzowany program sterujący Programowanie toru ruchu ściernicy dla szlifierki RUP 28 CNC moŝe odbywać się przez zastosowanie osi prostoliniowych w układzie prostokątnym lub biegunowym, natomiast programowanie ruchu z dodatkową osią C przez zadawanie współrzędnych końca ruchu osi C, X, Z lub przez zastosowanie funkcji TRANSMIT, co opisano w pozycjach [5, 6]. Na rysunku 7. wyjaśniono parametry przyjęte do opracowania programu obróbki typoszeregu części z rys. 5.
20 20 M. Krok, J. Porzycki, R. Wdowik W tabeli 1. przedstawiono opracowany program sterujący (główny i podprogram) przeznaczony do obróbki typoszeregu wyrobów określonych sparametryzowaną geometrią z rys. 7. dla szlifierki RUP 28 CNC z układem Sinumerik 840Di. Rys. 7. Rysunek pomocniczy do opracowania programu obróbki Fig. 7. Auxilary draft to work out of machining program Tabela 1. Program główny %_N_PROG_MPF oraz podprogram %_N_PROG_SPF Table 1. Main program %_N_PROG_MPF and subprogram %_N_PROG_SPF %_N_PROG_MPF EXTERN CYCLE_CAM(REAL,REAL,REAL,REAL,REAL,REAL,REAL,REAL,REAL,REAL) G54 WORKPIECE(,,,"CYLINDER",0,0,-20,-10,30) T="CUTTER" ;T="PLUNGE_CUTTER_3 A" ;T="ROUGHING_T80 A" SETMS(3) S4000 M3 CYCLE_CAM(-1,13,1,13,1,0,0.01,2,4000,10) SPOS=90 M30 %_N_PROG_SPF N10 PROC CYCLE_CAM(REAL _LEVEL, REAL _RAD1, REAL _LENG1, REAL _RAD2, REAL _LENG2, REAL _ANG, REAL _AP, REAL _ALLOW, REAL _FEEDR, REAL _SAVEL) SAVE ; DEFINICJA CYKLU WRAZ Z TYPEM ORAZ NAZWĄ PRZYJMOWANYCH PARAMETRÓW: ; _LEVEL - POZYCJA W OSI WZDŁUśNEJ ; _RAD1, _RAD2 - PROMIENIE ZAOKRĄGLENIA KRZYWKI ; _LENG1, _LENG2 - POŁOśENIA ŚRODKÓW OKRĘGÓW KRZYWKI
21 Parametryczne projektowanie szlifowania 21 ; _ANG - KĄT SKRĘCENIA KRZYWKI WZGLĘDEM OSI X ; _AP - DOSUW NA OBRÓT ; _ALLOW - NADDATEK DO USUNIĘCIA ; _FEEDR - POSUW/ PRĘDKOŚĆ OBWODOWA PRZEDMIOTU OBRABIANEGO ; _SAVEL - ODLEGŁOŚĆ BEZPIECZNA N20 DEF AXIS _PLANE=Z N30 DEF AXIS _LIN=X N40 DEF AXIS _CIR=SP1 ; DEFINICJA OSI W PRZYPADKU ZASTOSOWANIA CYKLU NA INNEJ OBRABIARCE N50 DEF INT _NOP, _I ; DEFINICJA ZMIENNYCH POMOCNICZNYCH ; _NOP - LICZBA PRZEJŚĆ ; _I - LICZNIK WYKONANYCH PRZEJŚĆ N60 _I=0 ; KASOWANIE LICZNIKA _I N70 G17 ; WYBÓR PŁASZCZYZNY KOREKCJI N80 DIAMOF ; WYŁĄCZENIE WYMIAROWANIA W ŚREDNICACH N90 G0 AX[_PLANE]=_LEVEL N100 G0 AX[_CIR]=90 ; NAJAZD NA POZYCJĘ PRACY N110 F=_FEEDR ; USTAWIENIE POSUWU N120 _NOP=ROUND(_ALLOW/_AP) ; OBLICZENIE ILOŚCI PRZEJŚĆ N130 TRANSMIT ; WŁĄCZENIE TRANSFORMACJI OSI X, Y NA OSIE X, C N140 OFFN=(_AP*(_NOP-_I)) ; USTAWIENIE ODSUNIĘCIA OD KONTURU N150 G1 X=-(_SAVEL+_ALLOW+_LENG1) Y=_RAD2 G41 ; NAJAZD NA PROFIL N160 PROFILE: N170 MSG("POZOSTALO NR: " << (_NOP-_I)) ; WYŚWIETLENIE KOMUNIKATU INFORMACYJNEGO O POZOSTAŁEJ ILOŚCI PRZEJŚĆ N180 G1 X=_LENG2 Y=_RAD2 N190 G2 X=_LENG2 Y=-_RAD2 I=AC(_LENG2) J=AC(0) N200 G1 X=-_LENG1 Y=-_RAD1 N210 G2 X=-_LENG1 Y=_RAD1 I=AC(-_LENG1) J=AC(0) ; OBRÓBKA KONTURU N220 _I=_I+1 ; ZWIĘKSZENIE LICZNIKA N230 OFFN=(_AP*(_NOP-_I)) ; DOSUNIĘCIE DO KONTURU O _AP N240 REPEAT PROFILE P=_NOP ; POWTÓRZENIE PROFILU OKREŚLONĄ ILOŚĆ RAZY N250 G1 X=_SAVEL+_ALLOW+_LENG1 Y=_RAD2 G40 ; ODJAZD OD KONTURU N260 TRAFOOF ; WYŁĄCZENIE TRANSFORMACJI N270 M17 Aby sprawdzić program obróbki, naleŝy dokonać jego symulacji. Na rysunku 8. przedstawiono ekran układu Sinumerik 840Di, na którym jest widoczny tor ruchu punktu charakterystycznego ściernicy podczas symulacji obróbki jednego
22 22 M. Krok, J. Porzycki, R. Wdowik z przedmiotów ich typoszeregu. Na podstawie symulacji moŝna określić czas obróbki przedmiotu. Rys. 8. Ekran symulatora układu Sinumerik 840Di Fig. 8. Screen of Sinumerik 840Di simulator czas [s] element typoszeregu Rys. 9. Czas obróbki typoszeregu wyrobów Fig. 9. Time of machining of type dimension products
23 Parametryczne projektowanie szlifowania Analiza czasu obróbki WaŜnym czynnikiem podczas planowania produkcji danego wyrobu jest znajomość głównego czasu obróbki. Rysunek 9. przedstawia czas obróbki typoszeregu części (od M1 do M12) z rys. 6. dla tych samych parametrów technologicznych. Zmienny czas wynika z róŝnicy drogi, jaką przebędzie punkt charakterystyczny ściernicy względem przedmiotu obrabianego podczas obróbki poszczególnych przedmiotów za pomocą tego samego sparametryzowanego programu obróbkowego. 5. Podsumowanie Ceramika techniczna ze względu na swoje właściwości uŝytkowe coraz częściej znajduje zastosowanie jako materiał konstrukcyjny. Obróbka wyrobów z ceramiki nie jest jednak łatwa, gdyŝ materiał ten naleŝy do trudno obrabialnych. Z tego powodu szczególnie obróbka wykończeniowa jest realizowana za pomocą szlifowania z uŝyciem ściernic diamentowych. Wyroby ceramiczne o złoŝonej geometrii wymuszają takŝe stosowanie do ich obróbki zaawansowanych wieloosiowych maszyn CNC, dla których konieczne jest właściwe opracowanie programu sterującego. Zastosowanie programowania parametrycznego upraszcza program sterujący, skraca jego długość, a przede wszystkim umoŝliwia obróbkę typoszeregu wyrobów za pomocą tego samego programu z róŝnymi wartościami parametrów. Ten sposób programowania upraszcza równieŝ wyznaczanie czasu obróbki kaŝdego przedmiotu ze zbioru objętego typoszeregiem wyrobów, co ma znaczenie podczas planowania produkcji. Mimo doskonalenia róŝnych sposobów obróbki skrawaniem materiałów w stanie twardym, moŝna twierdzić, Ŝe szlifowanie nadal zachowuje zdolność konkurowania z nimi dzięki stałemu postępowi zachodzącemu w budowie ściernic, szlifierek i w stosowanych procesach . W odniesieniu do ceramiki technicznej po końcowym spieczeniu jest ona przykładem efektywnej techniki jej obróbki ubytkowej. Literatura  Manison P.: Technical ceramics tough benefits, World Pumps, May  Liang Y., Dutta S.P.: Application trend in advanced ceramic technologies, Technovation, 21 (2001),  Oczoś K.E.: Kształtowanie ceramicznych materiałów technicznych, Oficyna Wydawnicza Politechniki Rzeszowskiej, Rzeszów  Materiały informacyjne firmy CEREL,  Stryczek R., Pytlak B.: Elastyczne programowanie obrabiarek, Wydawnictwo Naukowe PWN, Warszawa   Porzycki J.: Modelowanie szlifowania osiowego zewnętrznych powierzchni walcowych, Oficyna Wydawnicza Politechniki Rzeszowskiej, Rzeszów 2004.
24 24 M. Krok, J. Porzycki, R. Wdowik PARAMETRIC PROGRAMMING OF GRINDING OF CERAMIC PRODUCTS WITH COMPLEX GEOMETRY A b s t r a c t Machining of technical ceramic products requires application of CNC machines which have predetermined technological possibilities, special grinding tools and properly made control programs. In this paper parametric programming of ceramic products machining using CNC grinding machine with C axis is described. Time analysis of machining of type dimension ceramic products with parametric geometry is also presented. Keywords: parametric programming, grinding, CNC grinding machine, ceramic products DOI: /rm
25 ZESZYTY NAUKOWE POLITECHNIKI RZESZOWSKIEJ Nr 284 Mechanika z. 84 (4/12) 2012 Andrzej SKRZAT Rzeszow University of Technology APPLICATION OF COUPLED EULERIAN-LAGRANGIAN APPROACH IN METAL FORMING SIMULATIONS Numerical simulations of materials forming processes require both powerful computers and advanced software. Large displacements assumed in the analysis usually cause convergence problems. In the Lagrangian approach (typical for solid bodies) a remeshing is frequently necessary. This extends the computations and decreases the convergence. In such cases the application of Euler approach (typical for fluid flows) is an practical alternative. In the Euler approach the finite elements mesh remains fixed, while material flows through it. There is no need for remeshing, therefore. In this paper selected results of coupled Eulerian-Lagrangian analysis are presented. A bent beam as the benchmark test and backward extrusion as an example of metal forming process are considered. Some models parts (tools) are described by updated Lagrangian formulation, other parts (material) are described by Eulerian approach. Obtained results of CEL analyses were compared to ones of the pure Lagrangian approach. Keywords: coupled Eulerian-Lagrangian, large displacements, metal forming 1. Introduction Lagrangian and Eulerian approaches are commonly used in simulations of large displacement problems of solid mechanics. Both formulations have their advantages and limitations. In the Total Lagrangian approach (TL) the initial configuration for the time t = 0 and the final state for the time t + t are considered. In the Updated Lagrangian approach (UL) the configurations for the time t + t are referred to the solution obtained for the time t (Fig. 1). Unfortunately, as the finite element mesh becomes distorted under the loading, the generation of completely new mesh is required more or less frequently. It causes convergence problems and extends the computation time. In such cases the Eulerian approach becomes more efficient than Lagrangian approach. In the Eulerian formulation the finite element mesh remains fixed, while material flows through it. There is no need for remeshing, therefore. In the ninetieths Lagrangian and Eulerian approaches were combined together in the new approach called coupled Eulerian-Lagrangian (CEL). The CEL method was initially applied to
26 26 A. Skrzat fluid-structure interaction problems. In Figure 2 the results of the water-filled bottle drop-test are presented. The bottle strikes the floor at a skew angle, with one of the bottom corners experiencing the initial impact. A simulation for the bottle accounts both the exterior forces on the bottle from the floor impact, as well as the interior forces of the water pushing against the bottle. Coupled Eulerian-Lagrangian approach may be also applied to metal forming problems. In Figure 3 presented are the results of Lagrangian and CEL rivet forming simulations. Rivets are designed to create permanent attachments between two or more Fig. 1. Reference frames for total Lagrangian and updated Lagrangian Fig. 2. The water-filled bottle drop-test (CEL model) a) b) Fig. 3. Equivalent plastic strains in the rivet forming simulation Lagrangian (a) and CEL (b) analyses
27 Application of coupled Eulerian-Lagrangian 27 sheets of material. After both ends of the rivet are compressed the diameter of the rivet body expands, pinching the sheets of material between the two ends of the rivet. The rivet is modeled by Eulerian elements while tools are Lagrangian elements. In both exemplary simulations Lagrangian and Eulerian elements are combined simultaneously in the same model. In the CEL analyses bodies that undergo large deformations are meshed with Eulerian elements, while stiffer bodies in the model are meshed with more efficient Lagrangian elements. 2. Overview of coupled Lagrangian-Eulerian formulation In the Eulerian description equations are written using spatial time derivatives. In the standard Lagrangian description material time derivatives are used. The relation between material and spatial time derivatives is: DΦ Dt Φ = + v ( Φ) (1) t where: Φ the arbitrary solution variable, v the material velocity. D Φ and Dt Φ t are the material and spatial time derivatives, respectively. The Lagrangian mass, momentum and energy conservation equations transferred into the Eulerian (spatial derivatives) conservation equations  are: ρ + v ( ρ ) + ρ v = 0 (2) t v 1 + v ( v) = ( σ) + b (3) t ρ e + v ( e) = σ : D (4) t where: ρ the density, σ the Cauchy stress, b the vector of body forces, e the strain energy, D the velocity strain. The Eulerian equations (2)-(4) can be written in the conservative forms: ρ + ( ρv) = 0 t (5)
28 28 A. Skrzat ρv + ( ρv v) = σ + ρb t (6) e ( ev ) σ : D t (7) The Eulerian governing equations (5)-(7) have the general form: ϕ + Φ = S t (8) where: Φ the flux function, S the source term. Operator splitting divides Eq. (8) into two equations solved sequentially : ϕ = S t ϕ + Φ = 0 t (9) (10) Eq. (9) contains the source term represents the Lagrangian step. Eq. (10) contains the convective term represents the Eulerian step. Graphical representation of the split operator is shown in Fig. 4. Fig. 4. Split operator for the CEL formulation To solve Eq. (10) the deformed mesh from Lagrangian step is moved to the Eulerian fixed mesh, and volume of material transported between adjacent elements is calculated. The Lagrangian solution variables (e.g. mass, stress, energy) are adjusted to account for the flow of the material between adjacent elements. For the Lagrangian step the principle of virtual work is applied :
29 Application of coupled Eulerian-Lagrangian 29 ρa δ u d v + σ : δε dv = t δ u ds + ρb δ u dv (11) V V S V where: δ u the virtual displacement, δ ε the virtual strain resulting from virtual displacements, a the spatial acceleration, and t the surface traction. In the Lagarangian step the updated Lagrangian formulation is suitable because the reference configuration (time t) is the current configuration in the Eulerian approach. Unfortunately, in general the configuration of the body at time t + t considered in Eq. (11) is unknown (unknown is the volume of integration and density which depends on the body deformations). Moreover, the Cauchy stress at time t + t cannot be obtained by adding to the Cauchy stress at time t the stress increment because the components of the Cauchy stress tensor change when material is subjected to a rigid body rotation. In practice other strain and stress measures have to be used in the principle of virtual displacements (11) the Green-Lagrange strain tensor and the second Piola-Kirchoff stress tensor . In order to calculate the material(s) occupation in the Eulerian mesh the volume fraction parameter (VF) is introduced . The initial VF estimation requires the reference volume associated with the fixed regular Eulerian mesh (Fig. 5). The bent beam presented in Fig. 6 is considered as the benchmark test. The beam is modeled by Eulerian elements. The initial occupation of beam in 3D space is defined by the reference volume. The Eulerian part of the model surreference volume Eulerian mesh Fig. 5. Reference volume for the volume fraction parameter estimation 3. Benchmark test the bent beam
30 30 A. Skrzat rounds entirely the beam volume including its later deformations. In Figure 6 one can see two bottom supports and the upper punch being used to apply the load to the beam. Bilinear elastic-plastic material is assumed for the beam. Typically such problems are solved by Lagrangian approach. The results of the CEL analysis are presented in Fig. 7. The beam deflection and the distribution of stress is similar to ones obtained in pure Lagrangian analysis (not presented here). Unfortunately, in presented CEL analysis all the beam edges are rounded. This is caused by course Eulerian mesh. As a rule, a fine grid resolution comparable with the average radius of geometry curvature is required in Eulerian analyses. External loads can never be applied directly to the Eulerian mesh contact analysis is the only way to apply a mechanical load Fig. 6. Bent beam model Fig. 7. Equivalent stress in the bent beam CEL analysis
31 Application of coupled Eulerian-Lagrangian 31 to Eulerian elements. In this test the load is applied to the beam by rigid tools. In the case of other type of loads (e.g. pressure, concentrated force, moment) aditional flexible parts have to be included in the analysis. Auxiliary Lagrangian flexible parts loaded by mechanical forces affect the Eulerian parts by contact interactions. 4. Coupled Eulerian-Lagrangian simulation of backward extrusion The backward extrusion is a forming process widely used for the manufacturing of solid and hollow parts. The punch strikes the blank extruding it upwards by means of applied high pressure. The analysis of the extrusion forming operations requires evaluation of process parameters such as force and energy consumption as well as the determination of the distribution of the major field variables e.g. plastic strains. Numerical simulations of the backward extrusion process can lead to reduction of forming forces and allow to improve the forming accuracy. Unfortunately, from the mechanical point of view such simulations are very sophisticated. Usually, the finite element mesh becomes very distorted under the load and frequent remeshing is necessary, therefore. Large displacements, contact interactions and remeshing might be the source of convergence problems in Lagrangian analysis. In such cases the Eulerian analysis in which the finite element mesh remains fixed might provide reliable results . The FEM model of the coupled Eulerian-Lagrangian analysis of the backward extrusion process is presented in Fig. 8. The die and recipient are assumed to be rigid bodies. In this simulation the die moves into the cylindrical recipient. Fig. 8. FEM model of backward extrusion
32 32 A. Skrzat The processed material is aluminum alloy at 450 C. The stress-plastic strain curve is obtained from  for Bodner-Partom material model. Assumed B-P material data are: D 0 = 10 4 s -1, Z 0 = 280 MPa, Z 1 = 647 MPa, Z 2 = 35 MPa, Z 3 = 80 MPa, m 1 = 0,182 MPa -1, m 2 = 3,7 MPa -1, r 1 = r 2 = 4, A 1 = 0,15, A 2 = 0,99, n = 1,9. The description of Bodner-Partom material model and its material data is available in . In numerical computations commercial ABAQUS program was used. In ABAQUS program the coupled Eulerian-Lagrangian analysis is restricted to three-dimensional dynamic explicit problems only. Obtained equivalent plastic strain distribution in the extruded bar is shown in Fig. 9. The plot of external work versus the displacement obtained from the simulation is typical for backward extrusion problems (Fig. 10). Fig. 9. Equivalent plastic strain distribution in the extruded bar Fig. 10. External work vs. displacement in backward extrusion
33 Application of coupled Eulerian-Lagrangian 33 Considered problem can be solved more efficiently by axisymmetric Lagrangian analysis. Presented results obtained by the CEL analysis are comparable with the results of appropriate Lagrangian analysis which are not presented here. The effectiveness and stability of the CEL analysis can be demonstrated on extrusion problems in which more complicated extruded shapes are considered. In Fig. 11 the non-symmetric skewed double-tee bar used in the aviation industry is presented. Numerical Lagrangian simulation of the extrusion of this profile provides extreme element distortions, and it is both very time consuming and unstable. Fig. 11. Special double-tee beam used in aviation industry Coupled Eulerian-Lagrangian extrusion analysis runs for this profile without any problems. The only limitation is the size of this task. Thin web of an I-beam provides generation of very small Eulerian elements material cannot flow through several elements in one time/load increment. Moreover, the dynamic explicit procedure applied here is conditionally stable, and requires very small time increments (of order 10-6 s) when small finite elements are used. This extends the computation time very much. To solve this problem powerful workstation (12 processors, 24 Gb of memory) run this problem over two weeks. However, computations based on purely Lagrangian approach even if possible for this sophisticated geometry, would take more time. The geometry of extruded element for early stage of the considered backward extrusion problem is presented in Fig. 12. It should be kept in mind that in ABAQUS post processor in the visualization of the CEL analyses all edges are (unfortunately) rounded. Presented preliminary simulation is useful in the estimation of the size of the problem, required memory and the computation time in numerical simulations of reversed extrusion of sophisticated-shape elements. Results of such simulations will also help in better design of dies.
34 34 A. Skrzat Fig. 12. Backward extrusion of an I-beam profile 5. Conclusion The coupled Eulerian-Lagrangian approach is a very useful tool for solving large displacement problems. Many tasks which are very hard-to-solve by Lagrangian approach can be successfully solved by the CEL analysis. The CEL solution procedure is very stable even for complicated shapes because the Eulerian finite element mesh remains fixed during analysis. The CEL analysis is restricted only to dynamics problems in which inertia forces are considered. In ABAQUS program only explicit integration of the governing equations is allowed. It limits the application of the CEL analysis to short-term problems. In the dynamic explicit approach the stable time increment is usually very small, thus the long-term analysis would require millions of load increments and in consequence would take weeks or even months on powerful workstations. Presented results are very promising. They are stable independently of the shape of extruded elements. The last presented example is very hard to solve by Lagrangian approach. It was efficiently solved by coupled Eulerian-Lagrangian approach. In the future research the results of computer simulations will be compared with the experimental data. In Department of Material Forming and Processing hundreds of backward extrusion tests have been made for various types of materials, different extruded shapes and various temperature. This valuable experimental information will help to select an appropriate material model in presented simulation simple bilinear elastic-plastic material model was used. One of the candidates is Bodner-Partom material model which allows to take simultaneously into consideration elastic and plastic effects, isotropic and kinematic hardening, visco-plasticity, creep and relaxation for a wide range of temperature. Application of BP material model in the commercial software (ABAQUS) requires writing user material procedure.
35 Application of coupled Eulerian-Lagrangian 35 References  Benson D.J., Okazawa S.: Contact in a multi-material Eulerian finite element formulation, Comput. Methods Appl. Mech. Engng., 193 (2004),  Benson D.J.: A mixture theory for contact in multi-material Eulerian formulations, Comput. Methods Appl. Mech. Engng., 140 (1997),  Bathe K.J.: Finite element procedures, Upper Saddle River  Belytschko T., Liu K.W., Moran B.: Non-linear Finite Element Analysis for continua and structures, New York  Al-Athel K.S., Gadala M.S.: Eulerian volume of solid (VOS) approach in solid mechanics and metal forming, Comput. Methods Appl. Mech. Engng., 200 (2011),  Gouveia B.P.P.A., Rodrigues J.M.C., Martins P.A.F.: Finite element modeling of cold forward extrusion using updated Lagrangian and combined Eulerian- Lagrangian formulations, J. Mat. Proc. Technol., (1998),  Bodner S.R.: Unified plasticity for engineering applications, New York Boston  Skrzat A.: Fuzzy logic application to strain-stress analysis in selected elasticplastic material models, Arch. Metall. Mater., 56 (2011), ZASTOSOWANIE SPRZĘśONEGO PODEJŚCIA EULERA-LAGRANGE A W SYMULACJACH PROCESÓW PRZERÓBKI PLASTYCZNEJ METALI S t r e s z c z e n i e Numeryczne symulacje procesów przeróbki plastycznej wymagają duŝej mocy komputerów oraz zaawansowanego oprogramowania. Uwzględnienie w analizie duŝych przemieszczeń jest wielokrotnie źródłem powaŝnych trudności dotyczących zbieŝności obliczeń. W przypadku sformułowania Lagrange a stosowanego standardowo w analizie odkształcalnych ciał stałych często konieczne jest generowanie zupełnie nowej siatki MES, tzw. remeshingu. WydłuŜa to niestety czas analizy i pogarsza jej zbieŝność. W takich przypadkach rozsądną alternatywą jest zastosowanie podejścia Eulera (typowego dla analizy przepływu płynów) do obliczeń duŝych deformacji ciał stałych. W podejściu Eulera siatka elementów skończonych pozostaje nieruchoma, a przez siatkę przepływa materiał. W tym przypadku nie zachodzi konieczność remeshingu i nie pogarsza się uwarunkowanie problemu w czasie trwania obliczeń. W niniejszej pracy przedstawiono przykładowe wyniki obliczeń numerycznych z zastosowaniem sprzęŝonego podejścia Eulera-Lagrange a. Jako zadanie testowe analizowano belkę zginaną, jako przykład procesu przeróbki plastycznej rozpatrywano zagadnienie wyciskania przeciwbieŝnego. Dla niektórych części modeli (narzędzia) stosowano sformułowanie Lagrange a, a dla pozostałych części (obrabiany materiał) sformułowanie Eulera. Uzyskane rezultaty porównywano z wynikami obliczeń, w których zastosowano podejście czysto Lagrange owskie. Słowa kluczowe: sprzęŝona analiza Eulera-Lagrange a, duŝe przemieszczenia, kształtowanie plastyczne metali DOI: /rm
37 ZESZYTY NAUKOWE POLITECHNIKI RZESZOWSKIEJ Nr 284 Mechanika z. 84 (4/12) 2012 Ján SLOTA Miroslav JURČIŠIN Technical University of Košice, Slovakia EXPERIMENTAL AND NUMERICAL ANALYSIS OF THE DEEP DRAWING PROCESS USING OPTICAL MEASURING SYSTEM In this paper optimization of the deep drawing process with using a modern photogrammetric measurement system is discussed. The results obtained from optical measuring are compared with the results of a numerical simulation. The numerical simulation of this process was performed using two commercial FEM codes, which use different time integration schemes. Various results are illustrated in the details, compared and discussed. Optimization of the deep drawing process can reduce the amount of product defects, production cost and can improve the quality of products. Keywords: deep drawing, numerical simulation, photogrammetric measurement system 1. Introduction The deep drawing process is nowadays frequently used manufacturing technology in the industrial sphere. Many factors influence on a procedure of the forming process. These factors include for example the holding force [1, 2]. In order to optimize this process, numbers of tests have to be done. Their results may predict problematic or critical areas of the final product. Due to this in the industrial practice, numerical simulations are often used and they are based on finite element method (FEM) analysis and different time integration schemes. The most known integration schemes are the static implicit and the dynamic explicit. There are many publications which claim that only the dynamic explicit time integration scheme is accurate [3-5] or only the static implicit scheme is accurate enough [6-8]. In explicit strategy the current time step is solved once, resulting from previous time step. Based on required accuracy a mesh is locally redefined and changed. The problem is not solved again, and the solving process is not iterated. The method is convenient for tasks where the solution does not change in time . Implicit strategy is in every time step starting from the previous time step and the mesh is generated using local refinement due to requiring
38 38 J. Slota, M. Jurčišin accuracy of the problem, which is calculated on the current mesh. This solving process is iterated until the estimated error is between the bounds of an interval and requiring precision. If the time step between a new iteration is not too large, the time of the solving process is usually very small . The results of the numerical simulation may be compared with the ARGUS photogrammetric measuring system. The ARGUS is the contactless measuring system that on the basis of optical scanning allows predicting critical areas which take place during the forming process. On the sheet metal, a grid of circle points is etched before forming. The size of these points is between 1 and 6 mm. The grid is deformed at the same time as the sheet metal is deformed. The grid of circle points is deformed by the influence of direction and intensity of stresses, and its shape is changed. The measurement depends on the photogrammetric principle where the surface of a stamped part is scanned using a CCD camera in high resolution. Pictures are taken from different angles, and 3D coordinates of grid points are computed using image processing. Distances between points of the grid are defined by lateral distortion. On the basis of law of volume preservation distributions of major and minor strains, thickness reduction or critical areas of the drawn part are computed. Based on the defined material, forming limit diagram (FLD) is plotted . After all points are recognized, the 3D model of the drawn part is rendered, and analysis of strains, stresses, the thickness over a section can be performed. There are several studies which dealt with the similar problems [11, 12]. The material of a blank defined in the numerical simulation was in the case of a yield function approximated using Hill 48 yield function which is defined by the following law [13, 14]: ( ij ) F ( ) G ( ) H ( ) ϕ σ = σ σ + σ σ + σ σ + + 2Lσ + 2Mσ + 2Nσ σ = 0 (1) where: Φ(σ ij ) stress components with respect to the coordinate system, F, G, H, L, M, N Hill s anisotropic parameters, which can be expressed by a normal anisotropy, σ 22, σ 33, σ 11, σ 23, σ 31, σ 12 plane stresses; suffix 1 is parallel to the rolling direction, 2 is parallel to the transverse direction, σ scaling factor. 0 0 F, G, H, N ( ) ( r0 + r90 )( 1+ 2r45 ) ( ) r 1 r = = = = r r + 1 r + 1 r + 1 2r 1+ r (2)
39 Experimental and numerical analysis 39 where: r 0, r 45, r 90 values of the normal anisotropy measured in directions 0, 45 and 90 respectively to the rolling direction, L, M coefficients which are equal to the N. A hardening curve was defined by values obtained experimentally and subsequently approximated with the Hockett-Sherby material model . 2. Objectives and approach The aim of the experiment was to carry out the simulation of the deep drawing process in the explicit and implicit commercial software and then the results are compared with the real shape of a target product measured using the ARGUS optical measuring system. Mechanical properties of the mild steel DC05 are shown in the Table 1 and the target shape and the picture taken from the ARGUS measuring process are shown in the Fig. 1. The thickness of the blank was 0.8 mm. Table 1. Mechanical properties of the mild steel DC05 Specimen orientation R p0.2 [MPa] R m [MPa] A 80 [%] n C [MPa] where: R p0.2 yield stress, R m ultimate strength, A 80 total elongation, n strain hardening exponent, C strain coefficient, r normal anisotropy r a) b) Fig. 1. Shape of the drawn part in FEM code (a) and measured in ARGUS system (b)
40 40 J. Slota, M. Jurčišin The punch, die and blankholder shown in the Fig. 2 were modeled in the CAD software and exported to each of FEM code. Simulation was performed in the Autoform and PAM-STAMP code. A shell element type with a different number of integration points was used. In the case of the explicit code the number of integration points was 5, and 11 in case of the implicit code. The implicit code uses a triangular mesh type with angles of 30, and explicit code uses a rectangular mesh type with the size of 9.7 mm. The size of the element after refinement was equal to 1.2 mm. Stages defined in both FEM codes are shown in the Table 2. Table 2. Stages defined in the implicit and explicit code No Stage/Code Implicit Explicit 1 Positioning yes yes 2 Holding yes yes 3 Drawing yes yes 4 Springback yes yes 5 Cutting yes no The measurement of deformations, thickness reduction and 3D shape by the ARGUS optical measuring system was performed in the way as it was described in the previous chapter. Distances between centers of circles on the grid etched on the sheet were 1.5 mm. The results of the numerical simulation and the ARGUS measuring system will be described in the following chapter. a) b) Fig. 2. Assembly of tools in the FEM code (a) and the triangular refinement of the blank (b) 3. Results of experiment In order to compare differences between the results obtained from the ARGUS measuring system and numerical simulation, SVIEW software was
41 Experimental and numerical analysis 41 used. This comparison is necessary for interconnection of the model obtained from the FEM simulation and the model obtained from the ARGUS measuring system. All kind of inaccuracies defined in the numerical simulation can be found exactly by this comparison. The value of deviation between models is connected with the error of material model definition, the shape of tools and technological parameters defined in the numerical simulation. The deviation between models is showed in the Fig. 3. a) b) Fig. 3. Deviation of geometry of models obtained from ARGUS used explicit (a) and explicit (b) code Hence all parameters had the same value in the case of using the explicit and implicit codes, so comparison of these solvers could be discussed. It can be seen in the Fig. 3 that both codes showed similar deviation between models, but greater geometry deviation was observed in the case of implicit solver 2.93 mm in the absolute value. The absolute value of deviation when the explicit solver was used is 2.66 mm. The FLD diagram of the drawn part has a key role in the assessment of the technical process suitability. The FLD diagrams exported from FEM code and the ARGUS measuring system are showed in the Fig. 4 and 5. As it can be seen, neither in FEM code, nor in the ARGUS measuring system, none point is near or over forming limit curve. The FLD diagrams were exported for the bottom membrane of the part, because by using the ARGUS measuring system it is impossible to measure deformations or to obtain FLD in neutral membrane. Strain path of FLD is more suitable in the case of the explicit integration scheme as shown in the Fig. 5b. In the case of the ARGUS measuring system
42 42 J. Slota, M. Jurčišin some points in the area over 60% of major strain are visible, these points have not appeared in the FLD obtained from FEM codes. As it was mentioned, in the ARGUS measuring system a course of thickness reduction over section can be plotted. To analyze the accuracy of FEM code in comparison to ARGUS results, analysis of the thickness reduction was performed. The section through the drawn part was showed in the Fig. 6. The reason for selecting this section was that a few critical areas are near this section. This section was defined in both FEM models and the results were compared. major strain [%] minor strain [%] Fig. 4. FLD diagram obtained from ARGUS optical measuring system Distribution of thickness reduction over section is showed in the Fig. 7. In this picture distribution of thickness reduction obtained from the ARGUS measuring system and FEM simulations are presented. For better understanding and orientation, section over part is represented by broken line. As it can be seen in the Fig. 7, the ARGUS, and numerical simulations recognized the problematic areas in the same places. The greatest value of thickness reduction is observed in the bottom of the drawn part. On the left radius, both explicit and implicit codes overestimated the amount of the thickness reduction. On the right side of the drawn part, the thickness reduction was underestimated by the both FEM codes. In this case it is better to overestimate thickness reduction, because this can predict future defect. Smaller differences between numerical results and the ARGUS are observed on the right bottom radius (Fig. 7). The smallest amount of thickness reduction is observed on the bottom of the drawn part.
43 Experimental and numerical analysis 43 a) b) major strain (true strain) minor strain (true strain) Fig. 5. FLD diagram determined using implicit (a) and explicit (b) solver SECTION Fig. 6. Illustration of section over drawn part Fig. 7. Illustration of section over drawn part
44 44 J. Slota, M. Jurčišin 4. Conclusion Analyses of the deep drawing process using the ARGUS optical measuring system were discussed. Simulations were carried out using two different FEM codes and verified with results of experimental measurements. It can be concluded, that both codes had approximately the same results. Using this method it is possible to verify material models used to define blank behavior. It can be concluded that the results of the numerical simulation are accurate enough to predict critical areas of the drawn part. The same critical places of the drawn part were recognized with the ARGUS measuring system and both FEM codes. In the case of the FLD diagram there were no points over the forming limit curve. Considering the fact that implicit code needs less computing time according to explicit code, and the results varied about small values, it can be concluded that the implicit code is more convenient to use. Moreover, the implicit code needs less parameters which have to be defined, and needs less time spending with definition. Using the ARGUS optical measuring system leads to prediction critical areas on the drawn part and to optimization of the whole deep drawing process. References  Ahmetoglu M., Altan T.: Deep drawing of round cups using variable blank holder force (BHF), Reoirt Bi, ERC/NSM-S, Engineering Research Centre for Net Shape Manufacturing, Ohio State University, Ohio  Obermeyer E.J., Majlessi S.A.: A review of recent advances in the application of blank holder force towards improving of the forming limits of sheet metal parts, J. Mat. Proc. Technol., 75 (1998),  Lig Y., Tan M.J., Liew K.M.: Springback analysis for sheet forming processes by explicit finite element method in conjunction with the orthogonal regression analysis, Int. J. Solids and Structures, 36 (1999),  Yang D.Y., Jung D.W., Song I.S., Yoo D.J., Lee J.H.: Comparative investigation into implicit, explicit, and iterative implicit/explicit schemes for the simulation of sheet-metal forming processes, J. Mat. Proc. Technol., 50 (1995),  Jung D.W.: Static-explicit finite element method and its application to drawbead process with springback, J. Mat. Proc. Technol., 128, 1-3 (2002),  Meinders T. et.al.: A sensitivity analysis on the springback behavior of the unconstrained bending problem, J. Mat. Proc. Technol., 9, 3 (2006),  Li K., Geng L., Wagoner R.H.: Simulation of springback: Choice of element, [in:] Advanced technology of plasticity, M. Geiger (ed.), vol. 3, Springer-Verlag, Nuremberg 1999,  Hu Y.: Quasi-static finite element algorithms for sheet metal stamping springback simulation, Proc. of 4th Int. Conference and Workshop on Numerical Simulation of 3D Sheet Forming Processes, NUMISHEET 1999, J.C. Gelin and P. Picart (eds.),
45 Experimental and numerical analysis 45  Schmidt A., Kunibert G.S.: Design of adaptive finite element software. The finite element toolbox, Springer-Verlag, Bremen  ARGUS USER GUIDE,  Frącz W., Stachowicz F., Pieja T.: Aspect of verification and numerical optimization of sheet metal and numerical simulations process using the photogrammetric system, Acta Metallurgica Slovaca, 19 (2013) (in press).  Solfronk P., Sobotka J.: Utilization of forming tool with variable blankholder force for drawing of al alloys, Physics Procedia, 22 (2011),  Réche J., Besson J., Sturel T., Lemoine X., Gourgues-Lorenzon A.F.: Analysis of the air-bending test using finite-element simulation: Application to steel sheets, Int. J. Mech. Sci., 57 (2012),  Roll K.: Simulation of sheet metal forming Necessary developments in the future, Int. Conf. NUMISHEET 2008, Interlaken, Switzerland 2008,  AUTOFORM user guide, This contribution is the result of projects implementation: Center for research of control of technical, environmental and human risks for permanent development of production and products in mechanical engineering (ITMS: ) supported by the R&D Operational Programme funded by the ERDF and VEGA 1/0396/11. ANALIZA EKSPERYMENTALNA I NUMERYCZNA PROCESU GŁĘBOKIEGO TŁOCZENIA ZA POMOCĄ OPTYCZNEGO SYSTEMU POMIAROWEGO S t r e s z c z e n i e Wyniki otrzymane z zastosowaniem optycznego systemu pomiarowego zostały porównane z wynikami symulacji numerycznych. W artykule przedstawiono optymalizację procesu głębokiego tłoczenia z wykorzystaniem nowoczesnego fotogrametrycznego systemu pomiarowego. Symulacja numeryczna tego procesu została wykonana za pomocą dwóch komercyjnych programów MES z uŝyciem róŝnych schematów całkowania czasu. RóŜne wyniki zostały szczegółowo zilustrowane, porównane i omówione. Optymalizacja procesu głębokiego tłoczenia moŝe zmniejszyć liczbę wad wyrobu i koszt produkcji oraz poprawić jakość wyrobów. Słowa kluczowe: głębokie tłoczenie, symulacja numeryczna, fotogrametryczny system pomiarowy DOI: /rm
47 ZESZYTY NAUKOWE POLITECHNIKI RZESZOWSKIEJ Nr 284 Mechanika z. 84 (4/12) 2012 Roman ŠÚŇ Emil SPIŠÁK Technical University in Košice, Slovakia EVALUATION OF THE CUTTING EDGE FAN-SHAPED DURING THE CUTTING PROCESS BY THE HYDRO ABRASIVE WATER JET This article presents the current state of hydro-erosion cutting and factors affecting the quality of cutting surface. The aim of this article is the evaluation of the fanshaped water spray pattern on the bottom cut edge by the hydro-erosion cutting based on selected parameters like cutting surface roughness and the distance between the inlet and outlet water jet. The results demonstrate that cutting speed had the largest influence on evolution of fan-shaped bottom of the cut edge because increasing cutting speed increases the values of both parameters mentioned above. Keywords: hydro-erosion cutting, cutting speed, fan-shape, cutting surface quality 1. Introduction The cutting process of the material by the high pressure hydro abrasive water jet consists in removing a material by the mechanic effect of a narrow abrasive water jet at a high rate. The abrasive is used to increase the rate and the final quality of the cut material process . High rate hydro abrasive water jet is generated by means of a hydraulic pump creating high pressure water that is by means of mm diameter water jet cutter transformed into high rate water. The water jet penetrates the workpiece, gradually loses its kinetic energy and skews . The place where the water jet comes into contact with the cut material, gives rise to the reduction of the cut material by the controlled process. The result of such a process is a continuously cut material. Regarding the fact that a cut material is predominantly an abrasive with water, in the place where the material is cut, traces of the water jet effect in the cut direction and movement are visible. These traces of the water jet effect can be eliminated or even removed by the change of cutting parameters. Quality degrees of the surface topography introduced by KMT firm are also used in this article and are stated in five categories (Table 1).
48 48 R. Šúň, E. Spišák Table 1. Quality degrees of the surface topography Degree Characteristic Roughness Ra HK [µm] Roughness Ra DK [µm] Q1 dividing cut Q2 rough cut Q3 middle cut Q4 quality cut Q5 best cut < Ra HK roughness in the top outline, Ra DK roughness in the bottom outline Factors characterising the surface created by hydro erosion (surface of the cut edge) in relation to the quality and productivity hydro erosion process are stated in three categories : 1) basic physical properties, 2) the technical factors influence effecting the hydro erosion process, 3) the technological factors influence on the hydro abrasive surface erosion. Analysis of these factors and dimensioning of their optimal setting have an important influence on the quality of the operation of the technological process and the surface made by hydro erosion. During the process of material cutting by the high rate hydro abrasive water jet, the form of the device water jet is changed . At a distance of entering the water jet the cut material, the diameter of the water jet is expanded and diverted from the originally perpendicular water jet from its own axle. The size of the shape change that can be called curvature primarily depends on the rate of the device movement and the thickness and mechanical properties of the cut material. Energy decrease, resistance of the cut material and the movement rate are the basic factors affecting the characteristic shape of the device (water jet) in the cutting material [5, 6]. The curvature of the water jet is made in the opposite direction in comparison to the movement of the cutting head. The increasing of the deflection angle of the leaving water jet against the entering water jet is manifested in the worsening of surface quality that is expressed in the roughness of a new made surface and perpendicularity deflection of the material cut edge in the perpendicular direction to the cutting direction. Position of the place where the water jet enters the processed material is not compatible with the place where the water jet leaves the material. The place of the leaving water jet lags the place of the entering water jet. The lagging of the lower part of the water jet in comparison to the upper part is designated as jet lag ; in the picture below (Fig. 1) designated as L. The size of the jet lag is in the region of tenth millimetre up to several dozen millimetres and is a natural sign of an economical cutting way [7, 8].
49 Evaluation of the cutting edge fan-shaped 49 Fig. 1. Trace deflection of cut flag 2. Material and testing In our research, test samples of stainless material STN , class AISI 304 were used. This material represents chromium-nickel steel and, as to the anti-corrosive materials, it is the second most frequently used kind of material thanks to its resistance to corrosion, its cold forming and good welding property. The chromium-nickel steel is resistant to water, humidity, edible acids and weaker organic and anorganic acids. Temperature strain of this steel amounts to 300 C. AISI 304 is well publishable and suitable to be used in operations of deep drawing, folding and curling. This material is also suitable for electric arc but unsuitable for blaze welding. Test samples with a depth of 15 mm were cut by the abrasive water jet device with a high pressure pump SL II 50K and two CNC X-Y tables of 3000 x 1500 mm, next AUTOLINE I cutting head and an abrasive (Bengal Bay Garnet). The other constants and parameters are stated in the tables. Test samples were cut in four phases:
50 50 R. Šúň, E. Spišák perforation of the sample, 10 mm length cut from the perforation point (for the measurement of the cut boundary), sample cutting in the shape of a square (sides marked as a, b, c, d), each edge is cut at a different rate (a = 50 mm/min, b = 75 mm/min, c = 100 mm/min, d = 125 mm/min. Samples were cut altogether and all diameters were written down into a collecting register of test samples cutting. 16 samples out of the total amount of 64 have been selected for the purposes of this study. The results of measuring and cutting have been recorded in the tables and evaluated with the help of graphs. For the evaluation of the fan-shaped of the cut edge by the hydro erosion, roughness measurements of the cut edge of samples and measurements of size distance between water jet entering and water jet leaving were carried out as representing parameters influencing the creation of the fan-shaped of the lower cut edge of the cut material. The following parameters have remained constant with each tested sample: abrasive Bengal Bay Garnet (Mesh 80), water pressure 300 MPa, abrasive jet ø 1.02 mm. With regard to the extensiveness of the experiment, not all factors are stated; not all factor influencing the final quality of the cut surface as well as other evaluated parameters such as edge fanshaped and cut depth. Selected samples have been divided into 4 groups, each group containing 4 samples: Group 1 amount of abrasive 100 g/min; distance of water jet from material is 5 mm. Group 2 amount of abrasive 150 g/min; distance of water jet from material is 3 mm. Group 3 amount of abrasive 200 g/min; distance of water jet from material is 3 mm. Group 4 amount of abrasive 250 g/min; distance of jet from material is 3 mm. The following parameters have remained constant with each tested sample: abrasive Bengal Bay Garnet (Mesh 80), water pressure 300 MPa, abrasive jet ø 1.02 mm. With regard to the extensiveness of the experiment, not all factors are stated; not all factor influencing the final quality of the cut surface as well as other evaluated parameters such as edge fan-shaped and cut depth (Figs. 2-5).
51 Evaluation of the cutting edge fan-shaped 51 Fig. 2. Surface view of selected test samples cut with abrasive amount of 100 g/min Fig. 3. Surface view of selected test samples cut with abrasive amount of 150 g/min Fig. 4. Surface view of selected test samples cut with abrasive amount of 200 g/min
52 52 R. Šúň, E. Spišák Fig. 5. Surface view of selected test samples cut with abrasive amount of 250 g/min 3. Evaluation of the cutting edge fan-shaped A digital calliper Powerfix Profi has been used to measure and evaluate the intruded length of jet. The sample has been optically evaluated and the distance has been measured, by means of a calliper, in the most accentuated place of water jet entering and leaving (Fig. 6). The values gained have been written down into tables and evaluated by means of graphs (Figs. 7-10). waterjet entering movement direction of the cutting head L waterjet leaving Fig. 6. Distance measurement between water jet entering and leaving As it is shown in Fig. 7, the distance between input and output beam at a constant amount of abrasive 100 g/min decreased with increasing cutting speed. This graph clearly shows that the cutting speed of 125 mm/min is the optimum choice and cutting speed of 75 mm/min is the worst possible because featheriness is the greatest. Next graph (Fig. 8) shows that a constant amount of abrasive at 150 g/min, the distance between the input beam and output beam
53 Evaluation of the cutting edge fan-shaped 53 appears as the best possible in cutting speed of 50 mm/min and the worst possible choice would be to use a cutting speed of 100 mm/min, because the featheriness is the largest. Graphic evaluation of a constant amount of abrasive of 200 g/min (Fig. 9) clearly shows that the best used cutting speed appears cutting speed of 50 mm/min, where the distance between input and output beam is minimum. Opposite, proportionally increasing of featheriness using higher cutting speeds, that the highest cutting speed, 125 mm/min seems like the worst possible because featheriness is the greatest. As in the previous graph, graphical evaluation at a constant amount of abrasive 250 g/min (Fig. 10) shows that the increasing proportion of featheriness is based on increasing speed. We can conclude that for this quantity of abrasives, the most appropriate cutting speed seems to be 50 mm/min and as the worst possible speed is 125 mm/min due to featheriness. L, mm L [mm] 6,00 4,00 2,00 0,20 mm 0,25 mm 0,30 mm 0,35 mm 0, cutting Cutting speed, [mm/min] Fig. 7. The distance between water jet entering and leaving L dependence on cutting speed and water jet diameter, with abrasive amount of 100 g/min L, mm L [mm] 6,00 4,00 2,00 0,20 mm 0,25 mm 0,30 mm 0,35 mm 0, Cutting cutting speed, [mm/min] Fig. 8. The distance between water jet entering and leaving L dependence on cutting speed and water jet diameter, with abrasive amount of 150 g/min
54 54 R. Šúň, E. Spišák L, mm L [mm] 6,00 4,00 2,00 0,20 mm 0,25 mm 0,30 mm 0,35 mm 0, Cutting cutting speed, [mm/min] Fig. 9. The distance between water jet entering and leaving L dependence on cutting speed and water jet diameter, with abrasive amount of 200 g/min L [mm] L, mm 6,00 4,00 2,00 0,20 mm 0,25 mm 0,30 mm 0,35 mm 0, Cutting cutting speed, [mm/min] Fig. 10. The distance between water jet entering and leaving L dependence on cutting speed and water jet diameter, with abrasive amount of 250 g/min 4. Evaluation of the cutting edge roughness Roughness measuring was realized by Mitutoyo SJ-301 roughness measurement. The middle value was evaluated for Ra roughness for each side of evaluated samples. Roughness was evaluated with follow results: 1. At constant amount of grit 100 g/min, machined surface roughness has increased with increasing cutting speed (Fig. 11). At a cutting speed of 50 mm/min roughness was soft and at a cutting speed of 125 mm/min the roughness was harder. Finally we can conclude that this is maximum cut because the minimum value of Ra was 6.3 µm. 2. The Figure 12 shows that a constant amount of grit 150 g/min used at low speeds it seems to have positive effect on the soft roughness. Conversely,
55 Evaluation of the cutting edge fan-shaped 55 once again it confirmed that the rising rate negatively affects the roughness. We can conclude that this is maximum cut because the minimum value of Ra was 6.3 µm. 3. Using a constant amount grit 200 g/min, that for a given amount of abrasive there is a significant difference in roughness between the lowest and highest cutting speed (Fig. 13). Again, cutting speed of 50 mm/min appeared to be optimal and cutting speed 125 mm/min appeared as inappropriate. We can conclude that this is maximum cut, because of the smallest value of Ra that is in the range 4.0 to 6.3 µm. 4. The Figure 14 clearly shows that a constant amount of abrasives 250 g/min appears again the lowest cutting speed 50 mm/min is optimal and cutting speed 125 mm/min as inappropriate. The highest values of the roughness but not as high as in the previous figures, when a smaller amount of abrasives was used. Nevertheless, we can conclude that this is maximum cut because the lowest value of Ra is in the range of 4.0 to 6.3 µm. roughness Roughness Ra [µm] Ra, µm ,20 mm 0,25 mm 0,30 mm 0,35 mm cutting Cutting speed speed, [mm/min] mm/min Fig. 11. The cutting edge roughness dependence on cutting speed and water jet diameter, at constant average abrasive nozzle ø1.02 mm, distance of nozzle from material 5 mm, abrasive quantity of 100 g/min Based on the evaluated results, it was found that the positive effect on the quality of the cutting edge has lower cutting speed and more abrasive. At a cutting speed of 50 mm/min abrasives and weights of 200 g/min, the roughness ranged from 5.69 to 8.82 microns, which appeared to be optimal ratio selected. Negative impact on the quality of the cutting edge is a cutting speed, 100 mm/min and 125 mm/min. Surface roughness at a cutting speed of 125 g/min abrasives and weights 150 g/min ranged between 18.2 to µm.
56 56 R. Šúň, E. Spišák roughness Roughness Ra [µm] Ra, µm ,20 mm 0,25 mm 0,30 mm 0,35 mm cutting Cutting speed speed, [mm/min] Fig. 12. The cutting edge roughness dependence on cutting speed and water jet diameter, at constant average abrasive nozzle ø 1.02 mm, distance of nozzle from material 3 mm, abrasive quantity of 150 g/min roughness Roughness Ra [µm] Ra, µm ,20 mm 0,25 mm 0,30 mm 0,35 mm Cutting cutting speed, speed mm/min [mm/min] Fig. 13. The cutting edge roughness dependence on cutting speed and water jet diameter, at constant average abrasive nozzle ø 1.02 mm, distance of nozzle from material 3 mm, abrasive quantity of 200 g/min 5. Conclusion Based on the evaluated results, it has been determined that the distance between water jet entering and water jet leaving decreased with the increasing abrasive amount and by following lower cutting rates. The increasing of a cutting rate negatively influences on the quality of the cut surface and the distance between water jet entering and water jet leaving, because the increasing of
57 Evaluation of the cutting edge fan-shaped 57 roughness Roughness Ra [µm] Ra, µm ,20 mm 0,25 mm 0,30 mm 0,35 mm cutting Cutting speed speed, [mm/min] Fig. 14. The cutting edge roughness dependence on cutting speed and water jet diameter, at constant average abrasive nozzle ø 1.02 mm, distance of nozzle from material 3 mm, abrasive quantity of 250 g/min a cutting rate increases also values of the mentioned parameters. As to the distance between water jet entering and water leaving, the abrasive amount of g/min at the rate of 50 mm/min is considered to be optimal, but outside this range the influence of the abrasive amount impacts negatively, primarily on water jet entering and water jet leaving that has a direct influence on the cut edge fan-shaped. As an acceptable fan-shaped is considered the one visible to the naked eye because the bottom edge of the cut surface is no more relatively straight then. References  Maňková I.: Progresívne technológie: Advanced methods of material removal, Vienala, Košice  Híreš O., Hatala M., Hloch S.: Delenie kovových materiálov okružnou pílou, vodným prúdom a plazmovým oblúkom, JIŘÍ PUSTINA, Ostrava  Kmec J.: Vplyv parametrov vodného lúča na povrch vytvorený hydroabrazívnou eróziou, Vienala, Košice  Sobotová L., Tkáčová J.: Progresívne technológie. Návody na cvičenia, TU, SjF, Košice  Wilkins R.J., Graham E.E.: An erosion model of waterjet cutting, ASME J. Engng. Industry, 115 (1993),  Fabianová J.: Význam skúmania vplyvu rezných parametrov pri rezaní vodným lúčom, Výrobné Inžinierstvo, 2 (2007), (online: /journal/pdf07/2-str-53-55).  Vasilko K., Kmec J.: Delenie materiálu, DATAPRESS, Prešov  Waterjet machining tolerances: Limits to tolerance (online: /index.php?option=com_content&task=view&id=185&itemid=54).
58 58 R. Šúň, E. Spišák OCENA WACHLARZOWATOŚCI KRAWĘDZI CIĘCIA PODCZAS PROCESU CIĘCIA STRUMIENIEM WODNO-ŚCIERNYM S t r e s z c z e n i e Artykuł przedstawia bieŝący stan wiedzy na temat erozyjnego cięcia strumieniem wody oraz prezentuje wskaźniki, które wpływają na jakość powierzchni przecięcia. Celem artykułu jest ocena wachlarzowatości dolnej krawędzi powierzchni przecięcia na podstawie wybranych parametrów, takich jak chropowatość powierzchni przecięcia i odległość pomiędzy wlotem i wylotem strumienia wody. Wyniki badań wskazują, Ŝe prędkość cięcia ma największy wpływ na rozwój wachlarzowatości dolnej krawędzi powierzchni przecięcia, poniewaŝ zwiększenie prędkości cięcia zwiększa wartość obu wymienionych parametrów. Słowa kluczowe: cięcie wodno-erozyjne, prędkość cięcia, wachlarzowatość, jakość powierzchni cięcia DOI: /rm
59 ZESZYTY NAUKOWE POLITECHNIKI RZESZOWSKIEJ Nr 284 Mechanika z. 84 (4/12) 2012 Tomasz TRZEPIECIŃSKI Rzeszow University of Technology ADVANCES IN SHEET METAL FORMING TECHNOLOGIES In the article the changes associated with construction of machines used in die and die-less sheet metal forming have been presented. The selected future directions of development in new technologies and machines for sheet metal forming taking into account modern blank holding systems in the process of deep drawing have been indicated. Also the tendencies in introduction of new technologies and modernization of presently used technologies in order to increase productivity have been discussed. Keywords: blankholder, blankholder system, deep drawing, sheet metal forming 1. Introduction The development of power transmission systems of modern machines results in replacement of mechanical drives by hydrostatic, electrical and hybrid drives. The control of technological machines for metal forming is based on computer numerical control (CNC) systems and programmable logic controllers (PLC) as well as digital linear actuators. Mechanical transport mechanisms are replaced by robots and manipulators with higher adaptivity. Together with development of hydraulic and pneumatic drives, servo drives and digital linear drives it is possible to optimize the operating space of machines and to decrease the material consumption index. The most important characteristics of CNC machines used in sheet metal forming compared to the conventional machines are: automatic control systems feedback with control computer, many axes numerically controlled, application of automatic tool changer systems and 3-axis automatic modular transport systems, automatic diagnostic systems of collision and errors of primary control program, application of servo drives and precise toothed bars allowing to minimize clearances.
60 60 T. Trzepieciński Introducing into the market new constructional solutions of machines is connected with analysis of raising expectation of dimensional accuracy of products, processing speed, forming forces as well as static and dynamic rigidity . Analysing the machine market over last few years it can be observed, that producers are concentrated on elastic adaptation of machines for industrial consumer needs . 2. Deep drawing The development of sheet metal forming presses is connected with growing requirements of automotive industry and is focused on improvement of material flow and modernization of press driver. Increasing of material flow rat is realized by connection of press lines by using robots and 3-axis transfer machines with modular transport systems . Presently used autogenous press lines are composed with autonomous systems of material supply, manipulation and transport of finished products . The CNC controlling in hydraulically driver forming presses enables regulation of forming force and speed of press ram in the whole range of slide motion. The servo drive of crank presses allows for selection of drawing characteristics with codominant lower energy-consumption compared to the classical drives. The introducing into the market servomotors coupled with programmable PLC controllers by SEYI enables modification of stamping process characteristics and it is possible to set up low rotational speed of crankshaft. The example of usage direct servo drive press SD series is pressing with programmable pulsating motion that reduces undesirable residual stresses in a drawpiece [5, 6]. The innovative compact design of the press frame is combined with its own motor design specially developed, low speed servomotor with high torque and low energy consumption. Combined with an easy-to-operate, free programmable control system, it is possible to achieve dramatically reduced power consumption, improve productivity and extend tool life by 5-10 times. Progress in sheet metal forming technology is also connected with development of new techniques and machines for sheet metal cutting . Modernization of sheet-metal forming presses is connected not only with development of traditional stamping methods but also there is the extensive growth of new machines using a multi-segmented flat and tapered blankholders , pulsatory and elastic blankholders , intelligent multi input multi output (MIMO) systems with numerically controlled blankholder force (BHF) [10, 11].
61 Advances in sheet metal forming technologies Progress in blankholder systems In the pulsating blankholder system the blankholder is subjected to a vibratory (pulsating) force. The metal flowing into the bottom die is subjected to intermittent pressure at a frequency of up to 20 Hz. The material flow much better under the blankholder without the disadvantages of an essential low hold-down force. Increase of pulsation amplitude of the blank holder leads to decrease of frictional resistance and has a decisive effect on drawpiece quality . Some researches [13, 14] concluded that the increase of the frequency of the vibration leads to increase in the drawability and also results in a general decrease in thinning in comparison to the constant BHF. A pulsatory blankholder scheme could lead to reduction of the friction forces between the blankholder and blank, without increasing the danger of wrinkling and rapture . The newest tendencies to minimize the punch force and increase in limiting draw ratios affected the development of friction-actuated blank-holding technique  and elastic (pliable) blankholders . Blank holding is induced by applying a pressure on the upper surface of the elastic ring plate, which upon deflection would conform to the flange surface . Application of elastically deformable thin plate instead of classical rigid blankholder aims at enhancing more uniform contact conditions nearly all over the flange zone in contrast to the contact at the outer rim of the flange which is dominant in the case of the conventional rigid blankholder. Present effort is made to develop effective optimization techniques and devices to control process parameters and optimize the blankholder schemes. Based on the punchless deep drawing process  a new eight segments flat blankholder device was proposed . This device is made by fitting four flat small wedges in the gaps between the four flat drawing segments. In the case of forming thin sheets, a crack was observed due to the localized intensive shear deformation at the boundaries between the drawing segments and the wedges. To eliminate this defect a friction aided deep drawing process using tapered blankholder divided into four segments was proposed . The blankholder is made by cutting a tapered steel blankholder into eight segments. It consists of a stationary base and eight tapered drawing segments that have similar planes of 5 taper angle (Fig. 1c). The drawing segments can slide in radial direction under a constant speed over the tapered surfaces of the stationary base. In the first drawing step, deformation starts when four facing segments move radially inward to the die opening in the A-direction as shown in Fig. 1a. The other four segments in the B-direction move in the reverse direction, i.e. downward and radial outward opposite to the drawing direction as shown in Fig. 1b. In the A-direction the blank sheet and the die are lifted up (Fig. 1b), while in the B-direction there is no contact between the sheet and segments (Fig. 1c).
62 62 T. Trzepieciński F 1 F 2 Fig. 1. Schematic of eight segments tapered blankholder (a) and schematic of die in motion (b, c) The flexible manufacturing system using multi-point forming (MPF) technology is an advanced digital tooling system for the automatic fabrication of 3D surface parts . The main characteristic of the deformation method is given by the active surface discrete design of the forming elements which are composed of a number of pins, vertically aligned, according with the geometry of the part . The surface tooling in reconfigurable multipoint forming (RMF) is based on the concept of a die continuous surface discrete approximation (Fig. 2a). Usage of multi-point dies (Fig. 2b) mounted on special multipoint press machine (Fig. 2c) allows to obtain drawpieces with higher shape precision and under the decreased forming force, compared to traditional deep drawing. Based on the MPF methodology, an innovative dieless tooling (DT) and jigless tooling (JT) system is being developed. The DT/JT system integrates the technology of MPF with the technology of computer-aided and computercontrolled manufacturing. Overcoming mass production problems following try-out, new press technologies continuously emerge as new techniques and ideas in sheet metal forming are considered in press design. Controlling the flow of sheet metal via controllable multi-cylinder blankholder actuators reduces die-try out time by cutting down on die work [23-25]. The application of multi-input multi-output (MIMO) stamping process controller especially in case of forming complex-geometry parts allows to apply the non-uniform BHF in different regions of the drawpiece [23, 26].
63 Advances in sheet metal forming technologies 63 Fig. 2. Reconfigurable surface tooling (a), multi-punch stamping die (b) and multipoint forming press machine YAM8-315 (c), prepared on the basis of [21, 23] The deep drawing processes usually were done in the double-acting presses (most often used) with two rams or in the single-acting presses with a cushion system in the press table. In some single-acting presses, hydraulic cylinders are installed at the four corner points of the press table. Each cylinder has its own proportional or servo valve so that specific BHF can be run over the stroke for each cylinder. The BHF is transmitted from the cushion plate to the blankholder by several cushion pins. Numerically controlled height-adjustable cushion pins in hydromechanical multipoint cushion system have been recently developed . Each cushion pin has its own load cell to monitor the BHFs, which are introduced to the blankholder. In the flexible die blankholder system the blankholder is made from a nylon-based thermoplastic material and designed with pyramid-shaped steel inserts (Fig. 3). The BHFs are introduced into the pyramidshaped steel inserts (top down), so there is a clear correspondence between the BHF and the pressure-influenced base area of the pyramid. Between the stiff steel inserts, the flexible plastic material acts like elastic links. Fig. 3. Multi-point blankholder, where: A 1 -A 3 flat surfaces, BHF (1- n) blankholder forces
STRUCTURE AND ENVIRONMENT ARCHITECTURE, CIVIL ENGINEERING, ENVIRONMENTAL ENGINEERING AND ENERGY No. 4/2014 vol. 6 PL ISSN 2081-1500 www.sae.tu.kielce.pl KIELCE UNIVERSITY OF TECHNOLOGY Contents MAREK ŁAGODA,
SPIS TREŚCI - CONTENTS Nauka i Technika Wei PENG, Hong-Zhong HUANG, Xiaoling ZHANG, Yu LIU, Yanfeng LI Reliability Based Optimal Preventive Maintenance Policy of Series-parallel systems...4 Stanisław LEGUTKO
RADA PROGRAMOWA PRZEWODNICZĄCY: prof. dr hab. dr h.c. mult. Czesław CEMPEL Politechnika Poznańska REDAKTOR NACZELNY: prof. dr hab. inż. Ryszard MICHALSKI UWM w Olsztynie prof. dr hab. inż. Jan ADAMCZYK
Leszek KUŚMIERZ Grzegorz PONIEWAŻ ANALIZA WPŁYWU MODYFIKACJI GEOMETRII KRAWĘDZI ELEMENTU OPOROWEGO PŁYTKI WAHLIWEJ NA WŁAŚCIWOŚCI STREFY KONTAKTU ANALYSIS OF THE INFLUENCE OF GEOMETRY MODIFICATION OF EDGE
prof. dr hab. in. Jan ADAMCZYK AGH w Krakowie dr in. Roman BARCZEWSKI Politechnika Pozna ska prof. dr hab. in. Walter BARTELMUS Politechnika Wroc awska prof. dr hab. in. Wojciech BATKO AGH w Krakowie prof.
CZASOPISMO INŻYNIERII LĄDOWEJ, ŚRODOWISKA I ARCHITEKTURY JOURNAL OF CIVIL ENGINEERING, ENVIRONMENT AND ARCHITECTURE JCEEA, t. XXX, z. 60 (1/13), styczeń-marzec 2013, s. 5-18 STRESZCZENIA Jacek ABRAMCZYK
Article citation info: STOECK, M., OSIPOWICZ, T. The use of Newton s method for interpolation in the bench testing of compression-ignition engine unit injector systems. Combustion Engines. 2014, 159(4),
SPIS TREŚCI CONTENT: 1. Aleksander MOCZAŁA: Rozwój systemów ERP... 1 2. Leif GOLDHAHN, Michael KAISER: Development of adaptable multimedia process descriptions for process planning and manufacturing via
MODERN MANAGEMENT REVIEW 2014 MMR, vol. XIX, 21 (1/2014) January-March STRESZCZENIA Małgorzata BARAN 1 Justyna STECKO 2 SYMULACYJNY MODEL PRODUKCJA-ZBYT W KONWENCJI METODY DYNAMIKI SYSTEMÓW PRZYPADEK PRZEDSIĘBIORSTWA
Roczniki Kolegium Analiz Ekonomicznych nr 29/2013 Ludosław Drelichowski University of Technology and Life Sciences in Bydgoszcz Grzegorz Oszuścik Softeem Sp. z o.o. of Bydgoszcz Evaluation of the efficiency
Lublin University of Technology Electrical Engineering and Computer Science Faculty I E E E Lublin University of Technology Institute of Electrical Engineering & Electrotechnologies Polish Society of Theoretical
nr 1/2011 (1) s o c i a l s p a c e j o u r n a l. e u Rzeszów 2011 półrocznik nr 1/2011 (1) semi-annual Rzeszów s o c i a l s p a c e j o u r n a l. e u Rada Programowa Editorial Board Pirkkoliisa Ahponen,
WSPÓŁCZESNE ZARZĄDZANIE Kwartalnik Środowisk Naukowych i Liderów Biznesu CONTEMPORARY MANAGEMENT QUARTERLY The Journal of Scientific Community and Business Leaders 1/2011 ISSN 1643-5494 RADA PROGRAMOWA
KWARTALNIK POLSKIEGO TOWARZYSTWA FIZJOTERAPII TOM 20 NR 1 2012 ISSN-1230-8323 QUARTERLY POLISH SOCIETY OF PHYSIOTHERAPY INDEXED IN: EMBASE/Excerpta Medica, Index Copernicus WROC³AW 2012 FIZJOTERAPIA Kwartalnik
Global and Russian Energy Outlook to 2040 CNG Safety Changing Perceptions into Reality IAA Nutzfahrzeuge in Hannover: LNG-Tankstellen Nowa Kia Soul LPG test PHOTO - bevezetem PLAY IT SAFE WITH NON HAZARDOUS
Redakcyjne/Editorial Od Redakcji Od Redakcji Listopad 2007 SILNIKI SPALINOWE COMBUSTION ENGINES Czasopismo naukowe Scientific Magazine Nr 2/2007 (129) PL ISSN 0138-0346 Wydawca/Editor: Polskie Towarzystwo
User s manual Instrukcja obsługi NMS Novus Management System NMS - User s manual ver. 1.22 TABLE OF CONTENT Table of content... 3 1. FOREWORD INFORMATION...6 1.1. Main characteristics... 6 1.2. Recommended
INFORMATYKA EKONOMICZNA BUSINESS INFORMATICS 1(31) 2014 Wydawnictwo Uniwersytetu Ekonomicznego we Wrocławiu Wrocław 2014 Redaktorzy Wydawnictwa: Elżbieta Macauley, Tim Macauley, Jadwiga Marcinek Redaktor
Project title: MERIT REPORT OF A LAUREATE TEAM PROGRAMME Mars: another planet to approach geoscience issues Reporting period: from 01.05.2014 to 31.10.2014 Period no. 7 Agreement No.: Laureate: TEAM/2011-7/9
The use of search techniques employing ground-penetrating radar in forensic medicine Andrzej Ossowski, Piotr Brzeziński, Jarosław Piątek, Barbara Potocka-Banaś, Tomasz Janus, Katarzyna Jałowińska, Mirosław
Environment Protection Engineering Vol. 32 26 No. 1 ALICJA SIUTA-OLCHA* THERMAL PROCESSES IN SOLAR DOMESTIC HOT-WATER SYSTEM The heating of working medium in the core elements of a solar domestic hot water